High density assembly of energetic molecules under the constraint of defected 2D materials
Yan, Qi-Long; Yang, Zhijian; Zhang, Xue-Xue; Lyu, Jie-Yao; He, Wei; Huang, Shi; Liu, Pei-Jin; Zhang, Chaoyang; Zhang, Qing-Hua; He, Guo-Qiang; Nie, Fu-De; Journal of Materials Chemistry A 7 (2019) 17806–; doi:10.1039/C9TA03990B

data_7237668
_publ_section_title
;
 High density assembly of energetic molecules under the constraint of
 defected 2D materials
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry A'
_journal_page_first              17806
_journal_paper_doi               10.1039/C9TA03990B
_journal_volume                  7
_journal_year                    2019
_chemical_formula_moiety         'C3 H6 N6 O6'
_chemical_formula_sum            'C3 H6 N6 O6'
_chemical_formula_weight         222.14
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2018-06-12
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2018-06-20 deposited with the CCDC.	2019-07-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.545(4)
_cell_length_b                   10.663(3)
_cell_length_c                   13.185(4)
_cell_measurement_reflns_used    2902
_cell_measurement_temperature    173
_cell_measurement_theta_max      26.346
_cell_measurement_theta_min      3.025
_cell_volume                     1623.1(9)
_computing_cell_refinement       'SAINT v8.34A (Bruker, 2013)'
_computing_data_reduction        'SAINT v8.34A (Bruker, 2013)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      173
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measurement_device_type  'Bruker APX-II CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0298
_diffrn_reflns_av_unetI/netI     0.0273
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7238
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.356
_diffrn_reflns_theta_min         3.025
_exptl_absorpt_coefficient_mu    0.173
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_correction_T_min  0.6678
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2014/5 (Bruker,2014/5) was used for absorption correction. wR2(int) was 0.0661 before and 0.0498 after correction. The Ratio of minimum to maximum transmission is 0.8959. The \l/2 correction factor is 0.00150.'
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.818
_exptl_crystal_description       block
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.306
_refine_diff_density_min         -0.288
_refine_diff_density_rms         0.074
_refine_ls_extinction_coef       0.082(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.108
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     137
_refine_ls_number_reflns         1645
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.108
_refine_ls_R_factor_all          0.0416
_refine_ls_R_factor_gt           0.0357
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0622P)^2^+0.3678P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1029
_refine_ls_wR_factor_ref         0.1084
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1427
_reflns_number_total             1645
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9ta03990b2.cif
_cod_data_source_block           mo_20180607-29_0m
_cod_original_cell_volume        1623.2(8)
_cod_database_code               7237668
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_max   0.986
_shelx_estimated_absorpt_t_min   0.961
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups
2.a Secondary CH2 refined with riding coordinates:
 C3(H3A,H3B), C2(H2A,H2B), C1(H1A,H1B)
;
_olex2_submission_special_instructions 'No special instructions were received'